Polyester Resin Final Page 1 of 5
CHOOSING THE RIGHT RESIN – POLYESTER RESIN
Polyester Resin is a liquid which will cure to a solid when the hardener is added.
It has been specially formulated to cure at room temperature. The hardener,
MEKP (Methyl Ethyl Ketone Peroxide) is added to cure, or harden the resin.
MEKP hardeners for polyester resin, often referred to as catalyst come in small
plastic tubes or bottles with graduated measurements marked on them.
Hardeners are measured in drops or fractions of teaspoons for most lay-up or
repair jobs. Do not over-catalyze or under-catalyze -- you may ruin the resin and
have to start again. Always consult the manufacturer’s instructions for mixing
the correct proportions of hardener to resin. Factors that will affect the hardening
time and working time are temperature, thickness of the application, quantities of
resin mixed per batch and humidity.
Polyester resins have a limited shelf life of one year. Therefore, be sure to
purchase fresh resin and try to use it within six months from the time you
purchased it. Never return mixed polyester resin, (that which has been
catalyzed), to the container of unmixed resin. Discard the unused catalyzed
There are two general types of polyester resin used for repair. Laminating /
Bonding Resin which cures to a tacky surface and Fiberglass / Marine Finish
Resin which cures to a non-tacky surface.
Laminating Resin (Evercoat 100560, 100561) is used for large repairs, for initial
coats on wood, or for multiple applications with fiberglass cloth or mat. This resin
is air-inhibited which means it will cure to a tacky finish and does not require
sanding between coats. This is desirable in laminating because the layers
adhere to each other better, and the tacky layer will hold the cloth or mat in
place. This product should not be used as a final coat unless measures are taken
to seal out the air during the curing process.
Marine and Fiberglass Resin (Evercoat 100552, 100553, 100554, 100517,
100518, 100519, 105498, 105499, 105501 and 105502) are non air-inhibited or
waxed resins. They are for the final coat. This resin cures with a hard, non-
tacky surface. When the catalyzed resin is applied as a final coat to the laminate
coats of resin, the wax rises to the top, sealing off the air and allows the resin to
cure to a hard finish, which can then be sanded, painted or gel-coated.
NOTE: Cannot be used with aluminum, redwood and/or close-grained
woods like oak or cedar. For redwood, cedar, oak or other oily or close
grained woods, Evercoat Everfix Epoxy (100642, 100643) will provide the
Do not use with Styrofoam.
Polyester Resin Final Page 2 of 5
POLYESTER RESIN REPAIR PROCESS
Preparing the Surface
Before applying make sure the surface is clean. Remove all grease, wax, dirt,
and other foreign material from repair area. Use a paint stripper or sand off any
paint. Wipe area clean with acetone or non-residual solvent.
If repairing a hole, cut or grind away all loose or damaged material. Sand several
inches beyond repair area and taper edge of hole. Tape a wax paper covered
piece of cardboard to the backside of the hole to be repaired. Cut Sea-Glass
Cloth or Mat to overlap repair area by at least 2”. If multiple layers of mat or cloth
are going to be used, make each layer slightly larger than the last.
NOTE: BOAT YARD, BOATER’S CHOICE and HARDWARE RESIN MUST BE
USED WITH FIBERGLASS CLOTH, MAT or TAPE. AS A FINISHING COAT,
PREMIUM MARINE RESIN SHOULD BE USED WITH FIBERGLASS MAT,
CLOTH OR TAPE OVER LAMINATING (BONDING) RESIN.
Mixing the Material
Add hardener to resin just before using and stir for one minute. Never mix more
than a quart at a time as it starts setting up in about 17 minutes and should not
be used after it starts to gel (harden).
Mix resin and hardener using the chart below:
Required Hardener per Amount of Resin
Per Fl. Oz. of
Per Quart of
Per Gallon of
12 drops of
11 cc. of
44 cc. of
Application should only be made on a completely dry surface. When applying
resin over wood, the first coat may soak in. Apply a second coat before laying
Sea-Glass Mat or Cloth.
Using a paint brush or plastic spreader, apply resin/hardener mixture to the Sea-
Glass mat or cloth. Work the resin into the fiberglass until the white fibers
disappear. Additional layers of mat or cloth can be applied before the mixture
gels. After the finish coat has cured the surface must be sanded before re-
coating or painting.
Polyester Resin Final Page 3 of 5
After the Resin Has Cured (Hardened)
Once the repair has cured (at least 6 hours) sand down excess resin and any
protruding fibers with 80-120 grit. Use Evercoat Formula 27 All Purpose Filler
(100570, 100571, 100572), or White Marine Filler (100574) to fill in any low spots
or surface irregularities.
Sand final surface with 180-grit before applying paints or gel coat.
Fiberglass cloth, mat, or tape must be used with polyester resin.
Use only enough resin to completely wet out the cloth or mat. Excess resin that has
“puddled” on top of the cloth or mat will eventually crack.
Never return resin mixed with hardener back into the container.
Use EvercoatAcetone to clean brushes, tools and equipment before resin gels.
If desired, use Evercoat Coloring Agents to tint the resin. Tinting may not yield the
exact color match. Coloring Agents should be added prior to catalyzation at a
maximum of 1 oz. per quart.
Excessive brushing or applying in direct sunlight can cause resin to cure tacky.
Mat 1.5 oz. per sq. ft. 40% 1.5x 60%
Cloth 5.5 oz. per sq.yd. 50% 1.0x 50%
Woven Roving 24 oz. per sq. yd. 60% 0.67x 40%
Alternate Mat/Cloth 30% 2.33x 70%
Mat & Woven Roving 40% 1.5x 60%
Clean all tools and brushes with Evercoat Acetone as soon as you are finished to
prevent resin from hardening on them.
Note: Polyester resins cannot be used to repair thermoplastics (i.e.
Tupperware® or molded toys). Thermoplastics include polyethylene,
polypropylene, acrylic, PVC, ABS.
Polyester Resin Final Page 4 of 5
POLYESTER RESIN VERSUS EPOXY RESIN
Polyester Resin Epoxy Resin
Flexural Strength Good Best
Tensile Strength Good Best
Elongation % Good Lowest
Water Absorption Good Lowest/Excellent
Hardness Good Best
Pot Life 4 – 7 Minutes 14 – 20 Minutes
Working Time 20 – 30 Minutes ½ - 6 Hours
Above Waterline Yes Yes
Below Waterline Yes Yes
Major Construction Yes Yes
General Repairs Yes Yes
Shelf Life 1-year 1 Year +
Catalyst MEKP 2-Part System(1:1 mix)
Cure Time 6 – 8 Hours 24 - Hours
TINTING: Only color agents made specifically for polyesters should be
used when tinting or coloring polyester resin. Any chemical
foreign to the polyester can interrupt the curing process and
damage properties. No more than 1 ounce of color agent to
a quart of resin should be added. Tinting the resin may not
yield an exact color match.
THINNING: We do not recommend thinning the product.
TROUBLESHOOTING: POLYESTER RESINS
Common problems with polyester resins:
Problem: Resin is sticky all over after hardener has been mixed
into the resin and proper cure time has elapsed.
CAUSE #1: Incorrect mixing ratio was used when combining resin and
hardener. Use 12 drops of hardener per ounce of resin;
11 cc of hardener per quart of resin or 44cc of hardener per
gallon of resin.
CURE: Scrape off as much of the uncured resin as you can. You
can use acetone to clean the surface of any residue of
uncured resin. Follow with an application of properly mixed
Problem: Resin is still tacky (a finger leaves a fingerprint) after
hardener has been mixed into the resin and proper cure
time has elapsed.
Polyester Resin Final Page 5 of 5
CAUSE #1: The clear Hardener (Catalyst) that comes with the resin can
lose some of its potency or power with time, and/or adverse
CAUSE #2: Finishing Resins contain wax which seals oxygen and
creates a hard cured surface. If used in direct sunlight the
wax may not form on the surface causing a tacky surface.
CAUSE #3: User may have selected the incorrect resin for the project.
CURE #1: If finish resin (top coat) is desired, make sure you don’t
purchase and use a laminating resin (un-waxed resin)
designed for multiple coats of application (Evercoat 100561,
100560 are laminating, un-waxed resins). This resin is
designed to remain tacky until a finish resin is applied.
CURE #2: Put a heat lamp on the repair area at 120ºF two feet away
from the surface for a period of 2 hours. If the resin does not
respond by hardening further, proceed to CURE #3.
CURE #3: Increase hardener amount by 50% of the required amount
on the can’s directions (18 drops of hardener per ounce of
resin, instead of 12 drops), or ask place of purchase for the
most recent shipment of hardener.
COVERAGE, CURE TIMES, APPLICATION SUGGESTIONS
@ 10 mils
Important Notes that
apply to ALL Polyester
160 sq, ft.
50 sq. ft.
layer of Sea
gel or sand
4 to 6
Will not adhere to
aluminum or close-
grained woods. For
these surfaces, use an
Boat Yard Resin:
160 sq, ft.
50 sq. ft.
layer of Sea
gel or sand
4 to 6
Must be used with
fiberglass material like
cloth, mat or tape. May
not cure properly when
used without the